The material structure described by Li5Nb2V3O10 is Caswellsilverite-derived structured and crystallizes in the triclinic P-1 space group. There are three inequivalent Li sites. In the first Li site, Li(1) is bonded to two equivalent O(3), two equivalent O(4), and two equivalent O(5) atoms to form LiO6 octahedra that share corners with two equivalent Li(2)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with two equivalent V(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with four equivalent Li(2)O6 octahedra, and edges with four equivalent Nb(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-9°. In the second Li site, Li(2) is bonded to one O(1), one O(4), two equivalent O(3), and two equivalent O(5) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent Nb(1)O6 octahedra, corners with three equivalent V(2)O6 octahedra,  an edgeedge with one V(1)O6 octahedra,  an edgeedge with one V(2)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Nb(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-11°. In the third Li site, Li(3) is bonded to one O(1), one O(3), one O(4), one O(5), and two equivalent O(2) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with three equivalent Nb(1)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(3)O6 octahedra, edges with two equivalent Nb(1)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-10°. Nb(1) is bonded to one O(1), one O(2), one O(4), one O(5), and two equivalent O(3) atoms to form NbO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(2)O6 octahedra, corners with three equivalent Li(3)O6 octahedra,  an edgeedge with one Nb(1)O6 octahedra,  an edgeedge with one V(1)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-10°. There are two inequivalent V sites. In the first V site, V(1) is bonded to two equivalent O(1), two equivalent O(2), and two equivalent O(4) atoms to form VO6 octahedra that share corners with two equivalent Li(1)O6 octahedra, corners with two equivalent Nb(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with two equivalent Nb(1)O6 octahedra, edges with four equivalent Li(3)O6 octahedra, and edges with four equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 5-6°. In the second V site, V(2) is bonded to one O(4), one O(5), two equivalent O(1), and two equivalent O(2) atoms to form VO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with three equivalent Li(2)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(2)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Nb(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-11°. There are five inequivalent O sites. In the first O site, O(1) is bonded to one Li(2), one Li(3), one Nb(1), one V(1), and two equivalent V(2) atoms to form OLi2NbV3 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra, corners with two equivalent O(5)Li4NbV octahedra,  an edgeedge with one O(1)Li2NbV3 octahedra, edges with two equivalent O(3)Li4Nb2 octahedra, edges with two equivalent O(5)Li4NbV octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(2)Li2NbV3 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the second O site, O(2) is bonded to two equivalent Li(3), one Nb(1), one V(1), and two equivalent V(2) atoms to form OLi2NbV3 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(3)Li4Nb2 octahedra,  an edgeedge with one O(3)Li4Nb2 octahedra, edges with two equivalent O(2)Li2NbV3 octahedra, edges with two equivalent O(5)Li4NbV octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(1)Li2NbV3 octahedra. The corner-sharing octahedral tilt angles range from 0-8°. In the third O site, O(3) is bonded to one Li(1), one Li(3), two equivalent Li(2), and two equivalent Nb(1) atoms to form OLi4Nb2 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(2)Li2NbV3 octahedra,  an edgeedge with one O(2)Li2NbV3 octahedra, edges with two equivalent O(1)Li2NbV3 octahedra, edges with two equivalent O(3)Li4Nb2 octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(5)Li4NbV octahedra. The corner-sharing octahedral tilt angles range from 0-10°. In the fourth O site, O(4) is bonded to one Li(1), one Li(2), one Li(3), one Nb(1), one V(1), and one V(2) atom to form OLi3NbV2 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(4)Li3NbV2 octahedra, edges with three equivalent O(1)Li2NbV3 octahedra, edges with three equivalent O(2)Li2NbV3 octahedra, edges with three equivalent O(3)Li4Nb2 octahedra, and edges with three equivalent O(5)Li4NbV octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the fifth O site, O(5) is bonded to one Li(1), one Li(3), two equivalent Li(2), one Nb(1), and one V(2) atom to form OLi4NbV octahedra that share  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(1)Li2NbV3 octahedra,  an edgeedge with one O(5)Li4NbV octahedra, edges with two equivalent O(1)Li2NbV3 octahedra, edges with two equivalent O(2)Li2NbV3 octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(3)Li4Nb2 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. is represented by the CIF card [CIF]
data_Li5Nb2V3O10
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.240
_cell_length_b   5.259
_cell_length_c   7.920
_cell_angle_alpha   72.448
_cell_angle_beta   71.877
_cell_angle_gamma   79.007
_symmetry_Int_Tables_number   1
_cell_volume   196.619
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.500  1.000  0.500  1.0
  Li  Li1  1  0.228  0.482  0.596  1.0
  Li  Li2  1  0.772  0.518  0.404  1.0
  Li  Li3  1  0.396  0.489  0.214  1.0
  Li  Li4  1  0.604  0.511  0.786  1.0
  Nb  Nb5  1  0.091  0.992  0.323  1.0
  Nb  Nb6  1  0.909  0.008  0.677  1.0
  O  O7  1  0.049  0.751  0.145  1.0
  O  O8  1  0.951  0.249  0.855  1.0
  O  O9  1  0.328  0.251  0.062  1.0
  O  O10  1  0.672  0.749  0.938  1.0
  O  O11  1  0.161  0.252  0.454  1.0
  O  O12  1  0.839  0.748  0.546  1.0
  O  O13  1  0.228  0.749  0.754  1.0
  O  O14  1  0.772  0.251  0.246  1.0
  O  O15  1  0.432  0.767  0.344  1.0
  O  O16  1  0.568  0.233  0.656  1.0
  V  V17  1  1.000  0.500  0.000  1.0
  V  V18  1  0.694  0.005  0.099  1.0
  V  V19  1  0.306  0.995  0.901  1.0
[/CIF]
.
The material structure described by Li5Nb2V3O10 is Caswellsilverite-derived structured and crystallizes in the triclinic P-1 space group. There are three inequivalent Li sites. In the first Li site, Li(1) is bonded to two equivalent O(3), two equivalent O(4), and two equivalent O(5) atoms to form LiO6 octahedra that share corners with two equivalent Li(2)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with two equivalent V(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with four equivalent Li(2)O6 octahedra, and edges with four equivalent Nb(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-9°. In the second Li site, Li(2) is bonded to one O(1), one O(4), two equivalent O(3), and two equivalent O(5) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent Nb(1)O6 octahedra, corners with three equivalent V(2)O6 octahedra,  an edgeedge with one V(1)O6 octahedra,  an edgeedge with one V(2)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Nb(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-11°. In the third Li site, Li(3) is bonded to one O(1), one O(3), one O(4), one O(5), and two equivalent O(2) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with three equivalent Nb(1)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(3)O6 octahedra, edges with two equivalent Nb(1)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-10°. Nb(1) is bonded to one O(1), one O(2), one O(4), one O(5), and two equivalent O(3) atoms to form NbO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(2)O6 octahedra, corners with three equivalent Li(3)O6 octahedra,  an edgeedge with one Nb(1)O6 octahedra,  an edgeedge with one V(1)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-10°. There are two inequivalent V sites. In the first V site, V(1) is bonded to two equivalent O(1), two equivalent O(2), and two equivalent O(4) atoms to form VO6 octahedra that share corners with two equivalent Li(1)O6 octahedra, corners with two equivalent Nb(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with two equivalent Nb(1)O6 octahedra, edges with four equivalent Li(3)O6 octahedra, and edges with four equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 5-6°. In the second V site, V(2) is bonded to one O(4), one O(5), two equivalent O(1), and two equivalent O(2) atoms to form VO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with three equivalent Li(2)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(2)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Nb(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 3-11°. There are five inequivalent O sites. In the first O site, O(1) is bonded to one Li(2), one Li(3), one Nb(1), one V(1), and two equivalent V(2) atoms to form OLi2NbV3 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra, corners with two equivalent O(5)Li4NbV octahedra,  an edgeedge with one O(1)Li2NbV3 octahedra, edges with two equivalent O(3)Li4Nb2 octahedra, edges with two equivalent O(5)Li4NbV octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(2)Li2NbV3 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the second O site, O(2) is bonded to two equivalent Li(3), one Nb(1), one V(1), and two equivalent V(2) atoms to form OLi2NbV3 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(3)Li4Nb2 octahedra,  an edgeedge with one O(3)Li4Nb2 octahedra, edges with two equivalent O(2)Li2NbV3 octahedra, edges with two equivalent O(5)Li4NbV octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(1)Li2NbV3 octahedra. The corner-sharing octahedral tilt angles range from 0-8°. In the third O site, O(3) is bonded to one Li(1), one Li(3), two equivalent Li(2), and two equivalent Nb(1) atoms to form OLi4Nb2 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(2)Li2NbV3 octahedra,  an edgeedge with one O(2)Li2NbV3 octahedra, edges with two equivalent O(1)Li2NbV3 octahedra, edges with two equivalent O(3)Li4Nb2 octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(5)Li4NbV octahedra. The corner-sharing octahedral tilt angles range from 0-10°. In the fourth O site, O(4) is bonded to one Li(1), one Li(2), one Li(3), one Nb(1), one V(1), and one V(2) atom to form OLi3NbV2 octahedra that share  a cornercorner with one O(1)Li2NbV3 octahedra,  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(4)Li3NbV2 octahedra, edges with three equivalent O(1)Li2NbV3 octahedra, edges with three equivalent O(2)Li2NbV3 octahedra, edges with three equivalent O(3)Li4Nb2 octahedra, and edges with three equivalent O(5)Li4NbV octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the fifth O site, O(5) is bonded to one Li(1), one Li(3), two equivalent Li(2), one Nb(1), and one V(2) atom to form OLi4NbV octahedra that share  a cornercorner with one O(2)Li2NbV3 octahedra,  a cornercorner with one O(4)Li3NbV2 octahedra,  a cornercorner with one O(3)Li4Nb2 octahedra,  a cornercorner with one O(5)Li4NbV octahedra, corners with two equivalent O(1)Li2NbV3 octahedra,  an edgeedge with one O(5)Li4NbV octahedra, edges with two equivalent O(1)Li2NbV3 octahedra, edges with two equivalent O(2)Li2NbV3 octahedra, edges with three equivalent O(4)Li3NbV2 octahedra, and edges with four equivalent O(3)Li4Nb2 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. is represented by the CIF card [CIF]
data_Li5Nb2V3O10
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.240
_cell_length_b   5.259
_cell_length_c   7.920
_cell_angle_alpha   72.448
_cell_angle_beta   71.877
_cell_angle_gamma   79.007
_symmetry_Int_Tables_number   1
_cell_volume   196.619
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.500  1.000  0.500  1.0
  Li  Li1  1  0.228  0.482  0.596  1.0
  Li  Li2  1  0.772  0.518  0.404  1.0
  Li  Li3  1  0.396  0.489  0.214  1.0
  Li  Li4  1  0.604  0.511  0.786  1.0
  Nb  Nb5  1  0.091  0.992  0.323  1.0
  Nb  Nb6  1  0.909  0.008  0.677  1.0
  O  O7  1  0.049  0.751  0.145  1.0
  O  O8  1  0.951  0.249  0.855  1.0
  O  O9  1  0.328  0.251  0.062  1.0
  O  O10  1  0.672  0.749  0.938  1.0
  O  O11  1  0.161  0.252  0.454  1.0
  O  O12  1  0.839  0.748  0.546  1.0
  O  O13  1  0.228  0.749  0.754  1.0
  O  O14  1  0.772  0.251  0.246  1.0
  O  O15  1  0.432  0.767  0.344  1.0
  O  O16  1  0.568  0.233  0.656  1.0
  V  V17  1  1.000  0.500  0.000  1.0
  V  V18  1  0.694  0.005  0.099  1.0
  V  V19  1  0.306  0.995  0.901  1.0
[/CIF]
.